CH 6: Fatigue Failure Resulting from Variable Loading


 Herbert Lynch
 2 years ago
 Views:
Transcription
1 CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture). However, most machine elements are subjected to varying or fluctuating stresses (due to the movement) such as shafts, gears, bearings, cams & followers,etc. Fluctuating stresses (repeated over long period of time) will cause a part to fail (fracture) at a stress level much smaller than the ultimate strength (or even the yield strength in some casses). Unlike static loading where failure usualy can be detected before it happens (due to the large deflections associated with plastic deformation), fatigue failures are usualy sudden and therefore dangerous. Fatigue failure is somehow similar to brittle fracture where the fracture surfaces are prependicular to the load axis. According to LinearElastic Fracture Mechanics (LEFM), fatigue failure develops in three stages:  Stage1: development of one or more micro cracks (the size of two to five grains) due to the cyclic local plastic deformation.  Stage2: the cracks progress from micro cracks to larger cracks (macro cracks) and keep growing making a smooth plateaulike fracture surfaces with beach marks.  Stage3: occurs during the final stress cycle where the remaining material cannot support the load, thus resulting in a sudden fracture (can be brittle or ductile fracture). Fatigue failure is due to crack formation and propagation. Fatigue cracks usually initiate at location with high stresses such as discontinuities (hole, notch, scratch, sharp corner, crack, inclusions, etc.). CH 6 Page 1 of 20
2 Fatigue cracks can also initiate at surfaces having rough surface finish or due to the presence of tensile residual stresses. Thus all parts subjected to fatigue loading are heat treated and polished in order to increase the fatigue life. Fatigue Life Methods Fatigue failure is a much more complicated phenomenon than static failure where much complicating factors are involved. Also, testing materials for fatigue properties is more complicated and much more time consuming than static testing. Fatigue life methods are aimed to determine the life (number of loading cycles) of an element until failure. There are three major fatigue life methods where each is more accurate for some types of loading or for some materials. The three methods are: the stresslife method, the strainlife method, the linearelastic fracture mechanics method. The fatigue life is usually classified according to the number of loading cycles into: Low cycle fatigue (1 N 1000) and for this low number of cycles, designers sometimes ignore fatigue effects and just use static failure analysis. High cycle fatigue (N>10 3 ): Finite life: from cycles Infinite life: more than 10 6 cycles The StrainLife Method This method relates the fatigue life to the amount of plastic strain suffered by the part during the repeated loading cycles. When the stress in the material exceeds the yield strength and the material is plastically deformed, the material will be strain hardened and the yield strength will increase if the part is reloaded again. However, if the stress direction is reversed (from tension to compression), the yield strength in the reversed direction will be smaller than its initial value which CH 6 Page 2 of 20
3 means that the material has been softened in the reverse loading direction. Each time the stress is reversed, the yield strength in the other direction is decreased and the material gets softer and undergoes more plastic deformation until fracture occurs. The strainlife method is applicable to Lowcycle fatigue. The Linear Elastic Fracture Mechanics Method This method assumes that a crack initiates in the material and it keeps growing until failure occurs (the three stages described above). The LEFM approach assumes that a small crack already exists in the material, and it calculates the number of loading cycles required for the crack to grow to be large enough to cause the remaining material to fracture completely. This method is more applicable to Highcycle fatigue. The StressLife Method This method relates the fatigue life to the alternating stress level causing failure but it does not give any explanation to why fatigue failure happens. The stresslife relation is obtained experimentally using Moore highspeed rotating beam test.  The test is conducted by subjecting the rotating beam to a pure bending moment (of a fixed known magnitude) until failure occurs. (Due to rotation, the specimen is subjected to an alternating bending stress)  The data obtained from the tests is used to generate the fatigue strength vs. fatigue life diagram which is known as the SN diagram.  The first point is the ultimate strength which corresponds to failure in half a cycle.  The alternating stress amplitude is reduced below the ultimate strength and the test is run until failure. The stress level and the number of cycles until failure give a data point on the chart.  The testing continues and each time the stress amplitude is reduced (such that the specimen will live longer) and new point is obtained. CH 6 Page 3 of 20
4  For steel alloys the lowcycle fatigue and the highcycle fatigue (finite and infinite) can be recognized as having different slopes. (they are straight lines but keep in mind it is a loglog curve)  For steels if we keep reducing the stress amplitude (for each test) we will reach to a stress level for which the specimen will never fail, and this value of stress is known as the Endurance Limit (S e ).  The number of stress cycles associated with the Endurance Limit defines the boundary between Finitelife and Infinitelife, and it is usually between 10 6 to 10 7 cycles. Steel and Titanium alloys have a clear endurance limit, but this is not true for all materials. For instance, Aluminum alloys does not have an endurance limit and for such materials the fatigue strength is reported at 5(10 8 ) cycles. Also, most polymers do not have an endurance limit. The Endurance Limit The determination of the endurance limit is important for designing machine elements that are subjected to Highcycle fatigue. The common practice when designing such elements is to make sure that the fatigue stress level in the element is below the endurance limit of the material being used. Finding the Endurance Limit using the rotating beam experiment is time consuming where it requires testing many samples and the time for each test is relatively long. Therefore they try to relate the endurance limit to other mechanical properties which are easier to find (such as the ultimate tensile strength). CH 6 Page 4 of 20
5 The figure shows a plot of the Endurance Limits versus Tensile Strengths for a large number of steel and iron specimens.  The graph shows a correlation between the ultimate strength and endurance limit for ultimate strengths up to 1400 MPa then the endurance limit seems to have a constant value.  The relationship between the endurance limit and ultimate strength for steels is given as: S e = { 0.5 S ut S ut 1400 MPa 700 MPa S ut > 1400 MPa The prime ( ) is used to denote that this is the endurance limit value obtained for the test specimen (modifications are still needed). Endurance Limit Modifications Factors Endurance limit is obtained from the rotating beam test. The test is conducted under closely controlled conditions (polished specimen of small size at a constant known temperature, etc.). It is not realistic to expect a machine element to have the exact same endurance limit value as that obtained from the rotating beam test because it has different conditions (size, surface finish, manufacturing process, environment, etc.) Thus some modification factors are used to correlate the endurance limit for a given mechanical element to the value obtained from tests: Size Temp. Misc. S e = k a k b k c k d k e k f S e Where, Finish Load Reliability CH 6 Page 5 of 20
6 S e : The endurance limit at the critical location of a machine element with the geometry and conditions of use. S e : The endurance limit obtained from the rotating beam test. k a k f : Modification factors (obtained experimentally). Surface Condition Factor (k a ) The rotatingbeam test specimens are highly polished. A rough surface finish will reduce the endurance limit because there will be a higher potential for crack initiation. The surface condition modification factor depends on the surface finish of the part (ground, machined, as forged, etc.) and on the tensile strength of the material. It is given as: k a = a S ut b Constants a & b depend on surface condition and are given in Table 62. Size Factor (k b ) The rotatingbeam specimens have a specific (small) diameter (7.6mm). Parts of larger size are more likely to contain flaws and to have more nonhomogeneities. The size factor is given as: For bending and torsion 1.24 d d 51 mm k b = { 1.51 d < d 254 mm where d is the diameter, and: k b = 1 for axial loading When a circular shaft is not rotating we use an effective diameter value instead of the actual diameter, where: d e = 0.37 d For other crosssections, d e is found using Table 63 (find A 0.95σ from table then solve for d e using eqn. 623). CH 6 Page 6 of 20
7 Loading Factor (k c ) The rotatingbeam specimen is loaded in bending. Other types of loading will have a different effect. The load factor for the different types of loading is: 1 bending k c = { 0.85 axial 0.59 torsion Temperature Factor (k d ) When the operating temperature is below room temperature, the material becomes more brittle. When the temperature is high the yield strength decreases and the material becomes more ductile (and creep may occur). For steels, the tensile strength, and thus the endurance limit, slightly increases as temperature rises, then it starts to drop. Thus, the temperature factor is given as: k d = (10 3 )T c (10 5 )T c (10 8 )T c (10 12 )T c 4 For 37 T c 540 C The same values calculated by the equation are also given in Table 64 where: k d = ( S T S RT ) Reliability Factor (k e ) The endurance limit obtained from testing is usually reported at mean value (it has a normal distribution with σ = 8% ). For other values of reliability, k e is found from Table 65. MiscellaneousEffects Factor (k f ) It is used to account for the reduction of endurance limit due to all other effects (such as Residual stress, corrosion, cyclic frequency, metal spraying, etc.). However, those effects are not fully characterized and usually not accounted for. Thus we use (k f = 1). CH 6 Page 7 of 20
8 Stress Concentration and Notch Sensitivity Under fatigue loading conditions, crack initiation and growth usually starts in locations having high stress concentrations (such as grooves, holes, etc.). The presence of stress concentration reduces the fatigue life of an element (and the endurance limit) and it must be considered in fatigue failure analysis. However, due to the difference in ductility, the effect of stress concentration on fatigue properties is not the same for different materials. For materials under fatigue loading, the maximum stress near a notch (hole, fillet, etc.) is: σ max = K f σ o or τ max = K fs τ o Where, σ o : is the nominal stress K f : is the fatigue stress concentration factor which is a reduced value of the stress concentration factor (K t ) because of the difference in material sensitivity to the presence of notches. and K f is defined as: max. stress in notched specimen K f = stress in notch free specimen Notch sensitivity (q) is defined as: q = K f 1 K t 1 or q shear = K fs 1 K ts 1 Thus, The value of q ranges from 0 to 1 q = 0 K f = 1 (material is not sensitive) q = 1 K f = K t (material is fully sensitive) K f = 1 + q(k t 1) or K fs = 1 + q shear (K ts 1) For Steels and Aluminum (2024) the notch sensitivity for Bending and Axial loading can be found from Figure 620 and for Torsion is found from Figure CH 6 Page 8 of 20
9 Alternatively, instead of using the figures, the fatigue stress concentration factor K f, can be found as: K f = K t 1 1+ a r The Neuber equation where, r : radius a : is a material constant known as the Neuber constant. For steels, a can be found using Eqns. 635a & 635b given in the text (note that S ut needs to be in ksi and a will be given in in ) For cast iron, the notch sensitivity is very low from 0 to 0.2, but to be conservative it is recommended to use q = 0.2 For simple loading, K f can be multiplied by the stress value, or the endurance limit can be reduced by dividing it by K f. However, for combined loading each type of stress has to be multiplied by its corresponding K f value. Fatigue Strength In some design applications the number of load cycles the element is subjected to is limited (less than 10 6 ) and therefore there is no need to design for infinite life using the endurance limit. In such cases we need to find the Fatigue Strength associated with the desired life. For the Highcycle fatigue ( ), the line equation is S f = an b where the constants a (y intercept) and b (slope) are determined from the end points (S f ) 10 3 and (S f ) 10 6 as: a = (S 2 f) 10 3 S e and b = log (σ f S e ) log (2N e ) S e is the modified Endurance Limit CH 6 Page 9 of 20
10 Where σ f is the True Stress at Fracture and for steels with H B 500, it is approximated as: σ f = S ut Mpa  (S f ) 10 3 can be related to S ut as: fraction of where f is found as: (S f ) 10 3 = fs ut f = σ f S ut ( ) b Using the above equations, the value of f is found as a function of S ut (using N e = 10 6 ) and it is presented in graphical form in Figure For S ut values less than 490 MPa, use f = 0.9 to be conservative If the value of (f) is known, the constant b can be directly found as: and a can be rewritten as: b = 1 3 log (fs ut S e ) a = (fs ut) 2 S e  Thus for 10 3 N 10 6, the fatigue strength associated with a given life (N) is: (S f ) N = an b and the fatigue life (N) at a given fatigue stress (σ) is found as: N = ( σ a ) 1 b Studies show that for ductile materials, the Fatigue Stress Concentration Factor (K f ) reduces for N < 10 6, however the conservative approach is to use K f as is. Example: For a rotatingbeam specimen made of 1050 CD steel, find: CH 6 Page 10 of 20
11 a) The endurance limit (N e =10 6 ) b) The fatigue strength corresponding to ( ) cycles to failure c) The expected life under a completely reversed stress of 400 MPa Solution: From Table A20 S ut = 690 MPa a) S e = 0.5(S ut ) = 345 MPa b) σ f = S ut = 1035 MPa b = log (σ f S e ) log(1035 = 345 ) log(2n e ) log( = ) f = σ f ( ) b = 1035 S ut 690 (2 103 ) = a = (fs ut) 2 S e = ( )2 345 OR, easier, from Figure 618: f Then, = MPa Note that no modifications are needed since it is a specimen: S e = S e a = (fs ut) 2 S e = ( )2 345 = MPa b = 1 3 log (fs ut ) = log (0.845 ) = S e (S f ) N = an b (S f ) = 982.4( ) (S f ) = MPa c) N = ( σ 1 1 a ) b 400 = ( ) = cycles CH 6 Page 11 of 20
12 Example: The two axially loaded bars shown are made of 1050 HR steel and have machined surfaces. The two bars are subjected to a completely reversed load P. a) Estimate the maximum value of the load P for each of the two bars such that they will have infinite life (ignore buckling). b) Find the static and fatigue factors of safety n s & n f for bar (B) if it is to be subjected to a completely reversed load of P = 50 kn. c) Estimate the fatigue life of bar (B) under reversed load of P = 150 kn (use f = 0.9) Solution: From Table A20 S ut = 620 MPa & S y = 340 MPa a) S e = 0.5(S ut ) = 310 MPa Modifying factors:  Surface factor: k a = a S b ut, from Table 62: a = 4.51, b = k a = 4.51(620) = Size factor: k b = 1 since the loading is axial  Loading factor: k c = 0.85 (for axial loading)  Other factors: k d = k e = k f = 1 Stress concentration (for bar B): From Figure A153 with w d = 1.2 & r d = 0.1 K t 2.38 The fatigue stress concentration factor: K f = 1 + q(k t 1) From Figure 620 for steel: q 0.81 K f = (2.38 1) = 2.12 Thus the maximum stress for each is, Bar (A): S e = k a k c S e = (0.821)(0.85)(310) = MPa Bar (B): (S e ) mod = S e = = MPa K f 2.12 And the maximum load P for each is, Bar (A): P max = (25 25) = N Bar (B): P max = (25 25) = N CH 6 Page 12 of 20
13 Note that the maximum load for bar (B) is smaller than that of bar (A) because of the notch. b) Static factor of safety n s : From Table A20: ε f = 0.15 Ductile material, thus stress concentration is not applicable. σ o = P = = 80 MPa A net n s = S y σ o = = 4.25 Fatigue factor of safety n f : n f = (S e) mod σ o or n f = S e (K f σ o ) = (2.12)(80) = 1.28 c) If we calculate the fatigue factor of safety with P = 150 kn we will find it to be less than one and thus the bar will not have infinite life. a = (fs ut) 2 ( )2 = = MPa S e b = 1 3 log (fs ut ) = log (0.9 S e ) = σ o = P = = 240 MPa A net σ = K f σ o = = MPa N = ( σ 1 1 a ) b = ( ) = cycles This gives more conservative results than dividing (S e ) by K f, and using σ o as is. CH 6 Page 13 of 20
14 Characterizing Fluctuating Stress In the rotatingbeam test, the specimen is subjected to completely reversed stress cycles (σ max = σ min ) In the case of the rotating shaft subjected to both radial and axial loads (such as with helical gears) the fluctuating stress pattern will be different since there will be a component of stress that is always present (due to the axial load). The following stress components can be defined for distinguishing different states of fluctuating stress: σ m : Mean or average stress, σ m = σ max+σ min 2 σ r : Stress range, σ r = σ max σ min σ a : Stress amplitude (half of the stress range), σ a = σ max σ min 2 For uniform periodic fluctuating stress, σ m & σ a are used to characterize the stress pattern. We also define: Stress ratio: R = σ min σ max Amplitude ratio: A = σ a σ m Some common types of fluctuating stress: Completely reversed stress: σ m = 0 σ a = σ max = σ min Repeated stress: Tension σ a = σ m = σ max /2 Compression σ m = σ min /2 CH 6 Page 14 of 20
15 General fluctuating stress: (nonzero mean) σ a σ m 0 Fatigue Failure Criteria for Fluctuating Stress When a machine element is subjected to completely reversed stress (zero mean, σ m = 0) the endurance limit is obtained from the rotatingbeam test (after applying the necessary modifying factors). However, when the mean (or midrange) is nonzero the situation is different and a fatigue failure criteria is needed. If we plot the alternating stress component (σ a ) vs. the mean stress component (σ m ), this will help in distinguishing the different fluctuating stress scenarios. When σ m = 0 & σ a 0, this will be a completely reversed fluctuating stress. When σ a = 0 & σ m 0, this will be a static stress. Any combination of σ m & σ a will fall between the two extremes (completely reversed & static). CH 6 Page 15 of 20
16 Different theories are proposed to predict failure in such cases: Yield (Langer) line: It connects S y on the σ a axis with S y on σ m axis. But it is not realistic because S y is usually larger than S e. Soderberg line: The most conservative, it connects S e on σ a axis with S y on σ m axis. σ a S e + σ m S y = 1 n Where ( n) is the design factor ASMEelliptic line: Same as Soderberg but it uses an ellipse instead of the straight line. ( nσ 2 a ) + ( nσ 2 m ) = 1 S e S y It fits experimental data better (see fig 625) Goodman line: It considers failure due to static loading to be at S ut rather than S y, thus it connects S e on σ a axis with S ut on σ m axis using a straight line. σ a S e + σ m S ut = 1 n Gerber line: Same as Goodman but it uses a parabola instead of the straight line. nσ a S e + ( nσ 2 m ) = 1 S ut It should be noted that S e is the modified endurance limit. The fatigue stress concentration factor (K f ) should be multiplied with both σ a & σ m for conservative results. The load line represents any combination of σ a and σ m, the intersection of the load line with any of the failure lines gives the limiting values S a and S m according to the line it intercepts. CH 6 Page 16 of 20
17 Modified Goodman (Goodman and Langer) It combines the Goodman and Langer lines. The slope of the loading line passing through the intersection point of the two lines is called the critical slope and it is found as: r crit = S a S m where S m = (S y S e )S ut S ut S e & S a = S y S m According to the slope of the load line (r = σ a σ m ), it could intersect any of the two lines: r > r crit 1 S a = rs es ut rs ut + S e & S m = S a r, n f = S a σ a = S m σ m = r < r crit 2 S a = rs y 1 + r & S m = S y 1 + r, n s = S a σ a = S m σ m = Where case 2 is considered to be a static yielding failure. 1 σ a + σ m S e Sut S y σ a + σ m If we plot the Modified Goodman on stress (σ) vs. mean stress (σ m ) axes we obtain the complete Modified Goodman diagram where it defines a failure envelope such that any alternating stress that falls inside the diagram will not cause failure. The Complete Modified Goodman Diagram CH 6 Page 17 of 20
18 Also, there are other modified criteria: GerberLanger (see Table 67) ASMEellipticLanger (see Table 68) Combination of Loading Modes The procedures presented earlier can be used for fatigue calculations for a component subjected to general fluctuating stress (or fully reversed stress, easier) under one of the three modes of loading; Axial, Bending or Torsion. For a component subjected to general fluctuating stress under combination of loading modes: The stress corresponding to each mode of loading is split into its alternating (σ a ) and midrange (σ m ) components. The fatigue stress concentration factor corresponding to each mode of loading is applied to the (σ a & σ m ) of that mode. An equivalent von Mises stress is calculated for the alternating and midrange components as: 2 (σ σ a ) axial a = [(K f ) (σ bending a ) bending + (K f ) axial 0.85 ] + 3 [(K fs ) (τ torsion a ) torsion ] 2 σ m = [(K f ) bending (σ m ) bending + (K f ) axial (σ m ) axial ] [(K fs ) torsion (τ m ) torsion ] 2 Note that alternating component of the axial load is divided by 0.85 (i.e., k c for axial loading). The endurance limit is calculated assuming the loading is bending (i.e., k c = 1). Finally, a fatigue failure criterion (Gerber, Goodman, ASMEelliptic, etc.) is selected and applied as usual. A road map summarizing all the important equations for the stresslife method is given in Sec page 338. CH 6 Page 18 of 20
19 Example: A 40 mm diameter bar has been machined from AISI1045 CD bar. The bar will be subjected to a fluctuating tensile load varying from 0 to 100 kn. Because of the ends fillet radius, K f = 1.85 is to be used. Find the critical mean and alternating stress values S a & S m and the fatigue factor of safety n f according to the Modified Goodman fatigue criterion. Solution: From Table A20 S ut = 630 MPa & S y = 530 MPa S e = 0.5(S ut ) = 315 MPa Modifying factors:  Surface factor: k a = 4.51(630) = (Table 62)  Size factor: k b = 1 since the loading is axial  Loading factor: k c = 0.85 (for axial loading)  Other factors: k d = k e = k f = 1 S e = k a k c S e = (0.817)(0.85)(315) = MPa Fluctuating stress: σ = F A, A = π 4 d2 = mm 2 σ max = = 79.6 MPa & σ min = 0 σ m o = σ max + σ min 2 = 39.8 MPa & σ a o = σ max σ min 2 = 39.8 MPa Applying K f to both components: σ m = K f σ m o & σ a = K f σ a o σ m = σ a = 1.85(39.8) = 73.6 MPa The plot shows that the load line intersects the Goodman line: S a = rs es ut rs ut + S e = 1(218.8)(620) 1(620) CH 6 Page 19 of 20
20 S a = MPa = S m n f = 1 S a σ a + σ or n m f = = S m σ a σ m S e Sut n f = = 2.21 See Example 612 from text CH 6 Page 20 of 20
different levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationFATIGUE TESTS AND STRESSLIFE (SN) APPROACH
FATIGUE TESTS AND STRESSLIFE (SN) APPROACH FATIGUE TESTING LOADING TEST MACHINES SPECIMENS STANDARDS STRESSLIFE APPEROACH SN CURVES MEAN STRESS EFFECTS ON SN BEHAVIOR FACTORS INFLUENCING SN BEHAVIOR
More informationME311 Machine Design
ME Machine Design Lecture 5: FullyReversing Fatigue and the SN Diagram W Dornfeld Oct26 Fairfield University School of Engineering Discovering Fatigue With the Industrial Revolution came the steam engine
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationDESIGN TO PREVENT FATIGUE
W H I T E P A P E R DESIGN TO PREVENT FATIGUE Overview In 1954, two crashes involving the world s first commercial airliner, the de Havilland Comet, brought the words metal fatigue to newspaper headlines
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationFATIGUE CONSIDERATION IN DESIGN
FATIGUE CONSIDERATION IN DESIGN OBJECTIVES AND SCOPE In this module we will be discussing on design aspects related to fatigue failure, an important mode of failure in engineering components. Fatigue failure
More informationFatigue Failure Due to Variable Loading
Fatigue Failure Due to Variable Loading Daniel Hendrickson Department of Computer Science, Physics, and Engineering University of Michigan Flint Advisor: Olanrewaju Aluko 1. Abstract Fatigue failure in
More informationFAILURE MODES and MATERIALS PROPERTIES. Component failures. Ductile and Brittle Fracture COMPONENT FAILURES. COMPONENT FAILURE MODES examples:
FAILURE MODES and MATERIALS PROPERTIES MECH2300  Materials Lecture 10 R. W. Truss Materials Engineering R.Truss@uq.edu.au COMPONENT FAILURES Structures lectures es on component es cause response in component
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationLecture 14. Chapter 81
Lecture 14 Fatigue & Creep in Engineering Materials (Chapter 8) Chapter 81 Fatigue Fatigue = failure under applied cyclic stress. specimen compression on top bearing bearing motor counter flex coupling
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationShaft Design. Shaft Design. Shaft Design Procedure. Chapter 12
Shaft Design Chapter 1 Material taken from Mott, 003, Machine Elements in Mechanical Design Shaft Design A shaft is the component of a mechanical device that transmits rotational motion and power. It is
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationChapter 7: Fatigue and Impact
Chapter 7: Fatigue and Impact All machine and structural designs are problems in fatigue because the forces of Nature are always at work and each object must respond in some fashion. Carl Osgood, Fatigue
More informationExperiment: Fatigue Testing
Experiment: Fatigue Testing Objectives  To demonstrate the use of the Instron servohydraulic testing machine for testing specimens subjected to cyclic (fatigue) loadings.  To analytically approximate
More informationProperties of Materials
CHAPTER 1 Properties of Materials INTRODUCTION Materials are the driving force behind the technological revolutions and are the key ingredients for manufacturing. Materials are everywhere around us, and
More informationDesign Analysis and Review of Stresses at a Point
Design Analysis and Review of Stresses at a Point Need for Design Analysis: To verify the design for safety of the structure and the users. To understand the results obtained in FEA, it is necessary to
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationMIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE
MIME 3330 Mechanics Laboratory LAB 5: ROTATING BENDING FATIGUE Introduction In this experiment, the finite life fatigue behavior of a smooth cylindrical specimen as shown in Figure 1 will be studied in
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationFatigue Failure Resulting from Variable Loading
bud21932_ch06_257345 09/02/2006 12:06 AM Page 257 CONFIRMING PAGES 6 Fatigue Failure Resulting from Variable Loading Chapter Outline 6 1 Introduction to Fatigue in Metals 6 2 Approach to Fatigue Failure
More informationLecture Slides. Chapter 10. Mechanical Springs
Lecture Slides Chapter 10 Mechanical Springs The McGrawHill Companies 2012 Chapter Outline Mechanical Springs Exert Force Provide flexibility Store or absorb energy Helical Spring Helical coil spring
More informationFatigue of Metals Copper Alloys. Samuli Heikkinen 26.6.2003
Fatigue of Metals Copper Alloys Samuli Heikkinen 26.6.2003 T 70 C Temperature Profile of HDS Structure Stress amplitude 220 MPa Stress Profile of HDS Structure CLIC Number of Cycles f = 100 Hz 24 hours
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationPROPERTIES OF MATERIALS
1 PROPERTIES OF MATERIALS 1.1 PROPERTIES OF MATERIALS Different materials possess different properties in varying degree and therefore behave in different ways under given conditions. These properties
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationFatigue Life Estimates Using Goodman Diagrams
Fatigue Life Estimates Using Goodman Diagrams by Robert Stone The purpose of this paper is to review the proper methods by which spring manufacturers should estimate the fatigue life of a helical compression
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS
EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationFATIGUE FROM VARIABLE AMPLITUDE LOADING. Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1
FATIGUE FROM VARIABLE AMPLITUDE LOADING Ali Fatemi  University of Toledo All Rights Reserved Chapter 9 Variable Amplitude Loading 1 FATIGUE FROM VARIABLE AMPLITUDE LOADING SPECTRUM LOADS AND CUMULATIVE
More informationSAMPLE FORMAL LABORATORY REPORT. Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas
SAMPLE FORMAL LABORATORY REPORT Fatigue Failure through Bending Experiment Adapted from a report submitted by Sarah Thomas Lab Partners: David Henry and James Johnson ME 498 November 10, 2004 Professor
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More informationMAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationMECHANICS OF MATERIALS
T dition CHTR MCHNICS OF MTRIS Ferdinand. Beer. Russell Johnston, Jr. John T. DeWolf ecture Notes: J. Walt Oler Texas Tech University Stress and Strain xial oading  Contents Stress & Strain: xial oading
More informationME 343: Mechanical Design3
ME 343: Mechanical Design3 Design of Shaft (continue) Dr. Aly Mousaad Aly Department of Mechanical Engineering Faculty of Engineering, Alexandria University Objectives At the end of this lesson, we should
More informationFatigue Analysis of an Inline Skate Axel
FATIGUE ANALYSIS OF AN INLINE SKATE AXEL 57 Fatigue Analysis of an Inline Skate Axel Authors: Faculty Sponsor: Department: Garrett Hansen, Mike Woizeschke Dr. Shanzhong (Shawn) Duan Mechanical Engineering
More informationDistinguishing strength from toughness. Understanding fracture toughness.
Lecture notes version 20 Oct 2010 Chapter 8 Fracture and fracture toughness A fractured Liberty Ship 8.1 Introduction and synopsis Distinguishing strength from toughness. Understanding fracture toughness.
More informationCompletely reversed, strain controlled fatigue tests of a steel alloy with E=210000 MPa resulted in the following data:
Kul49.4350 Fatigue o Structure Example solutions 5 Problem 51. Completely reversed, strain controlled atigue tests o a steel alloy with E=10000 resulted in the ollowing data: a a, (o the stable curve)
More informationPREVENTING MECHANICAL FATIGUE
TECHNICAL PAPER PREVENTING MECHANICAL FATIGUE Overview Fatigue is the most common cause of catastrophic failure in metals and can occur in other materials as well. SolidWorks software provides a fast,
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationFatigue crack propagation
1 (20) Repetition Ð Crack initiation and growth Small cracks Shear driven Interact with microstructure Mostly analyzed by continuum mechanics approaches Large cracks Tension driven Fairly insensitive to
More informationLecture 12: Fundamental Concepts in Structural Plasticity
Lecture 12: Fundamental Concepts in Structural Plasticity Plastic properties of the material were already introduced briefly earlier in the present notes. The critical slenderness ratio of column is controlled
More informationCalculating and Displaying Fatigue Results
Calculating and Displaying Fatigue Results The ANSYS Fatigue Module has a wide range of features for performing calculations and presenting analysis results. By Raymond Browell Product Manager New Technologies
More information2.75 6.525 Problem Set 1 Solutions to ME problems Fall 2013
2.75 6.525 Problem Set 1 Solutions to ME problems Fall 2013 2. Pinned Joint problem Jacob Bayless a) Draw a freebody diagram for the pin. How is it loaded? Does the loading depend on whether the pin is
More informationLecture Slides. Chapter 8. Screws, Fasteners, and the Design of Nonpermanent Joints
Lecture Slides Chapter 8 Screws, Fasteners, and the Design of Nonpermanent Joints The McGrawHill Companies 2012 Chapter Outline Reasons for Nonpermanent Fasteners Field assembly Disassembly Maintenance
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More information1.Adapted from Gordon, J.E., Structures or why things don t fall down, Da Capo Press, Inc., New York, N.Y., 1978, Chapter 15.
Lecture 4: Cyclic loading and fatigue Safe working life: 1 All structures will be broken or destroyed in the end just as all people will die in the end. It is the purpose of medicine and engineering to
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationWELD  STATIC AND FATIGUE STRENGTH III
32 WELD  STATIC AND FATIGUE STRENGTH III 1.0 INTRODUCTION A component or a structure, which can withstand a single application of load, may fracture if the same load is applied a large number of times.
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationEffects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 4140 Steel
Paper 281434 Effects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 414 Steel Copyright 28 SAE International Nisha Cyril and Ali Fatemi The University
More information2.1 CYCLIC/FATIGUE LOADING OF STRUCTURAL MEMBERS
CHAPTER TWO 2. CYCLIC/FATIGUE LOADING OF STRUCTURAL MEMBERS Quite a while ago, engineers discovered that if you repeatedly applied and then removed a nominal load to and from a metal part (known as cyclic
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationDamage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max
5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when
More informationPOWER SCREWS (ACME THREAD) DESIGN
POWER SCREWS (ACME THREAD) DESIGN There are at least three types of power screw threads: the square thread, the Acme thread, and the buttress thread. Of these, the square and buttress threads are the most
More informationMechanical properties 3 Bend test and hardness test of materials
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More informationThe factor of safety is a factor of ignorance. If the stress on a part at a critical location (the
Appendix C The Factor of Safety as a Design Variable C.1 INTRODUCTION The factor of safety is a factor of ignorance. If the stress on a part at a critical location (the applied stress) is known precisely,
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationModule 2 GEARS. Lecture 9  SPUR GEAR DESIGN
Module 2 GEARS Lecture 9  SPUR GEAR DESIGN Contents 9.1 Problem 1 Analysis 9.2 Problem 2 Spur gear 9.1 PROBLEM 1 SPUR GEAR DESIGN In a conveyor system a stepdown gear drive is used. The input pinion
More informationFailure Analysis of a Cast A380 Aluminum Alloy Casting Using a Microstructurally Based Fatigue Model
Failure Analysis of a Cast A380 Aluminum Alloy Casting Using a Microstructurally Based Fatigue Model C.L. Burton, M.K. Jones, D.L. Oglesby A.L. Oppedal, M.Q. Chandler, M.F. Horstemeyer Center for Advanced
More informationMachine Design II Prof. K.Gopinath & Prof. M.M.Mayuram. Module 2  GEARS. Lecture 17 DESIGN OF GEARBOX
Module 2  GEARS Lecture 17 DESIGN OF GEARBOX Contents 17.1 Commercial gearboxes 17.2 Gearbox design. 17.1 COMMERCIAL GEARBOXES Various commercial gearbox designs are depicted in Fig. 17.1 to 17.10. These
More information1.054/1.541 Mechanics and Design of Concrete Structures (309) Outline 1 Introduction / Design Criteria for Reinforced Concrete Structures
Prof. Oral Buyukozturk Massachusetts Institute of Technology Outline 1 1.054/1.541 Mechanics and Design of Concrete Structures (309) Outline 1 Introduction / Design Criteria for Reinforced Concrete Structures
More informationHow Management Decisions Make or Break Plant Uptime
How Management Decisions Make or Break Plant Uptime Abstract How Management Decisions Make of Break Plant Uptime: When you run machines above design rates that decision goes against all that we know about
More informationSPECIFICATIONS, LOADS, AND METHODS OF DESIGN
CHAPTER Structural Steel Design LRFD Method Third Edition SPECIFICATIONS, LOADS, AND METHODS OF DESIGN A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural
More informationMECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS COMPRESSION MEMBERS TUTORIAL 1 STRUTS You should judge your progress by completing the self assessment exercises. On completion of this tutorial you should be able to do the following.
More informationRESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE
RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE RESISTANCE Ali FatemiUniversity of Toledo All Rights Reserved Chapter 8 Residual Stresses & Their Effects 1 RESIDUAL STRESSES AND THEIR EFFECTS ON FATIGUE
More informationInvestigation Of Heat Treating Of Railroad Wheels And Its Effect On Braking Using Finite Element Analysis
Investigation Of Heat Treating Of Railroad Wheels And Its Effect On Braking Using Finite Element Analysis Kexiu Wang Richard Pilon Griffin Wheel Company Abstract This paper studies the heat treatment process
More informationB.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN
No. of Printed Pages : 7 BAS01.0 B.TECH. (AEROSPACE ENGINEERING) PROGRAMME (BTAE) CV CA CV C:) O TermEnd Examination December, 2011 BAS010 : MACHINE DESIGN Time : 3 hours Maximum Marks : 70 Note : (1)
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationShaft Design under Fatigue Loading By Using Modified Goodman Method
Shaft Design under Fatigue Loading By Using Modified Goodman Method R. A. Gujar 1, S. V. Bhaskar 2 1, 2 (Department of Mechanical Engineering, Pune University, Maharashtra ABSTRACT In this paper, shaft
More informationENGINEERING COUNCIL CERTIFICATE LEVEL
ENGINEERING COUNCIL CERTIICATE LEVEL ENGINEERING SCIENCE C103 TUTORIAL  BASIC STUDIES O STRESS AND STRAIN You should judge your progress by completing the self assessment exercises. These may be sent
More informationDesign. Lecturer. Mohammed Midhat Hasan (Teacher) MSc. Applied Mechanics. Main reference
Mechanical Engineering Design Lecturer (Teacher) MSc. Applied Mechanics University of Technology Department of Production Engineering and Metallurgy Main reference Shigley s Mechanical Engineering Design,
More information